SHANDONGHAANGLAS CO., LTD
HEAT FLOW METERTEST REPORTSCOPE OF WORKVIG SPECIMEN - 3S1.16+0.3V+3 - ASTM C518

REPORT NUMBER
P0492.01-116-25 R1TEST DATE
10/06/2022 to 10/12/2022
ISSUE DATE
10/21/22

REVISED DATE
11/2/2022

PAGES
12DOCUMENT CONTROL NUMBER
RT-R-AMER-Test-7906 (01/17/22)©2017 INTERTEK

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22REPORT ISSUED TO
SHANDONG HAANGLAS CO., LTD
NO.2 Dongyue Avenue
Tai'an,SECTION 1SUMMARYSERIES/MODEL: VIG Specimen - 3S1.16+0.3V+3
Architectural Testing, Inc. (an Intertek Company), dba Intertek Building & Construction (B&C),
was contracted by Shandong HaanGlas Co., Ltd to perform heat flow meter testing inaccordance with ASTM C518-21 on their, Vacuum Insulated Glass Unit. Results obtained aretested values and were secured by using the designated test method. Testing was conductedat the Intertek B&C test facility in York, Pennsylvania.

Intertek B&C is an accredited testing laboratory and all testing was conducted in fullcompliance with ASTM approved procedures and specifications.
Intertek B&C will service this report for the entire test record retention period. The test record
retention period ends four years after the test date. Test records, such as detailed drawings,
datasheets, or other pertinent project documentation, will be retained for the entire test
record retention period. This report does not constitute certification of this product nor anopinion or endorsement by this laboratory.

For INTERTEK B&C:
COMPLETED BY: Benjamin W. GreenREVIEWED BY:

TITLE:

Project Lead

TITLE:

Eric S. LeitnerManager - Thermal Testing& Simulations

SIGNATURE:
DATE:

11/02/22

SIGNATURE:
DATE:

11/02/22

BWG:bwg
This report is for the exclusive use of Intertek's Client and is provided pursuant to the agreement between Intertek and its Client.
Intertek's responsibility and liability are limited to the terms and conditions of the agreement. Intertek assumes no liability to any
party, other than to the Client in accordance with the agreement, for any loss, expense or damage occasioned by the use of thisreport. Only the Client is authorized to permit copying or distribution of this report and then only in its entirety. Any use of theIntertek name or one of its marks for the sale or advertisement of the tested material, product or service must first be approved inwriting by Intertek. The observations and test results in this report are relevant only to the sample(s) tested. This report by itself
does not imply that the material, product, or service is or has ever been under an Intertek certification program.

Version: 01/17/22

Page 2 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 2
TEST METHODS
The product were evaluated in accordance with the following:
ASTM C518-21, Standard Test Method for Steady-State Thermal Transmission Properties
by Means of the Heat Flow Meter Apparatus
SECTION 3
TEST SPECIMEN DESCRIPTIONSERIES/MODELPRODUCT TYPE
SPECIMEN TEST SIZEVIG Specimen - 3S1.16+0.3V+3Vacuum Insulated Glass Unit
12" x 12"*This product is not a compressible sample.

SPECIMEN CONSTRUCTION

The test specimens were provided by the client as 6 units
measuring approximately 1/4" x 12" x 12". Samples wereplaced into a foam surround mask of the same thickness,
instrumented with surface thermocouples located on thetop and bottom surfaces in the center of each panel. Thenthe samples were installed into the apparatus with buffermats between the meter and surfaces of each panel toensure proper contact with the apparatus. See Appendix B:Photographs.

SECTION 4
TEST CONDITIONSCOLD PLATE TEMPERATURE
WARM PLATE TEMPERATURE
MEAN SPECIMEN TEMPERATURE
AVERAGE TEMPERATURE GRADIENTHEAT FLOW ORIENTATIONSPECIMEN CONFIGURATIONMETERING AREA

Version: 01/17/22

10°F nominal
60°F nominal
35°F nominal
50°F/inch nominal
Vertical Heat Flow, The specimen was prepared andinstalled into the test apparatus horizontally so thatthe measured heat flow was from the hot plate to thecold plate, as intended for use.
Single horizontal specimen
4" x 4" heat flux transducer on warm side plate

Page 3 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 5
EQUIPMENTDESCRIPTION
Dial Calipers (0-12")
Adams Scale (CBK 70A)
Digital Indicators (0-1")
Temp/Humidity Transmitter
Intertek 24" HFMSERIAL #ASSET #
52-008-012-0
INT01848
17960300
65197
17960305
65196
12961265
63736
Y003323*Device calibrated prior to use.

CALIBRATION DATE01/18/23
12/15/22
01/14/23
02/24/23*SECTION 6CALIBRATION INFORMATION

Calibration Material

Material Thermal Conductance

NIST Standard Reference Material 1450d, 1" Thickness
Fibrous Glass Board, Serial Number 357, dated January 20,
2012, no expiration.
0.211(C) (Btu/hr·ft²·°F)

Test Specimen ID

Sample Name

Avg. Heat Flux
(Btu/hr·ft²)

Avg. Thermal
Conductance (C)(Btu/hr·ft²·°F)
Avg. Thermal
Resistance (R)(hr·ft²·°F/Btu)
Avg. Thermal
Resistivity (r)(hr·ft²·°F/Btu-in)
Apparent Thermal
Conductivity (k)(Btu-in/hr·ft²·°F)
Specimen Avg.
Thickness(inches)†Specimen Avg.
Density(Lbs./Ft3)

SECTION 7
TEST RESULTS (IP Units)

1

Sample 1

4.24

0.085

11.81

47.62

0.021

0.248

194.482

Sample 2

3.77

0.076

13.19

53.19

0.019

0.248

194.293

Sample 3

4.34

0.087

11.53

46.31

0.022

0.249

194.674

Sample 4

4.40

0.088

11.36

45.62

0.022

0.249

195.625

Sample 5

4.27

0.086

11.70

47.18

0.021

0.248

194.486

Sample 6

3.84

0.077

13.05

52.62

0.019

0.248192.71

Version: 01/17/22

Page 4 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22

Test Specimen ID

Sample Name

Avg. Heat Flux
(W/m²)

Avg. Thermal
Conductance (C)(W/m²·K)
Avg. Thermal
Resistance (Rsi)(m²·K/W)
Avg. Thermal
Resistivity (r)(m·K/W)
Apparent Thermal
Conductivity (k)(W/m·K)
Specimen Avg.
Thickness(mm)†Specimen Avg.
Density(kg/m³)

SECTION 7 (continued)
TEST RESULTS (SI Units)

1

Sample 1

13.36

0.481

2.08

330.17

0.003

6.30

3115.212

Sample 2

11.91

0.430

2.32

368.79

0.003

6.30

3112.163

Sample 3

13.69

0.492

2.03

321.09

0.003

6.32

3118.27

4

Sample 4

13.87

0.500

2.00

316.30

0.003

6.32

3133.52

5

Sample 5

13.48

0.485

2.06

327.12

0.003

6.30

3115.21

6Sample 6

12.11

0.435

2.30

364.84

0.003

6.30

3086.98†The density of the sample was determined by dividing the average weight of the sample by its volume. The
weight was measured using a calibrated scale and the volume was determined by measuring the length, width,and height of the sample.

ANSI/NCSL Z540-2-1997 Type B uncertainty for this test was:

Version: 01/17/22

Page 5 of 124%

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8
PICTURES
VIG Specimen - 3S1.16+0.3V+3, (Sample 1)

Version: 01/17/22

Page 6 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8 (continued)
PICTURES
VIG Specimen - 3S1.16+0.3V+3, (Sample 2)

Version: 01/17/22

Page 7 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8 (continued)
PICTURES
VIG Specimen - 3S1.16+0.3V+3, (Sample 3)

Version: 01/17/22

Page 8 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8 (continued)
PICTURES
VIG Specimen - 3S1.16+0.3V+3, (Sample 4)

Version: 01/17/22

Page 9 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8 (continued)
PICTURES
VIG Specimen - 3S1.16+0.3V+3, (Sample 5)

Version: 01/17/22

Page 10 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 8 (continued)
PICTURES
VIG Specimen - 3S1.16+0.3V+3, Unit (Sample 6)

Version: 01/17/22

Page 11 of 12

RT-R-AMER-Test-7906

130 Derry Court
York, PA, 17406
Telephone: 717-764-7700
Facsimile: 717-764-4129
www.intertek.com/building

TEST REPORT FOR SHANDONG HAANGLAS CO., LTD
Report No.: P0492.01-116-25 R1
Date: 11/02/22
SECTION 9
REVISION LOGREVISION #.01 R0.01 R1

Version: 01/17/22

DATE
10/21/22
11/02/22

PAGES
N/AAllREVISION
Original Report Issued to Customer.
Corrected Syntax Error

Page 12 of 12

RT-R-AMER-Test-7906